Organic-Inorganic Hybrid Materials: Hydrothermal Syntheses and Structural Characterization of Bimetallic Organophosphonate Oxides of the Type Mo/Cu/O/RPO32-/Organoimine
Robert C. Finn; Randy S. Rarig; Jon Zubieta; Inorganic Chemistry 41 (2002) 2109–2123; doi:10.1021/ic011124v

data_4317880
_publ_section_title
;
 Organic-Inorganic Hybrid Materials: Hydrothermal Syntheses and Structural
 Characterization of Bimetallic Organophosphonate Oxides of the Type
 Mo/Cu/O/RPO32-/Organoimine
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2109
_journal_page_last               2123
_journal_paper_doi               10.1021/ic011124v
_journal_volume                  41
_journal_year                    2002
_chemical_formula_sum            'C11 H14 Cu Mo2 N2 O13 P2'
_chemical_formula_weight         699.60
_chemical_name_systematic
;
  ?
;
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   7.8280(11)
_cell_length_b                   19.877(3)
_cell_length_c                   25.460(4)
_cell_measurement_temperature    293(2)
_cell_volume                     3961.5(10)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.985
_diffrn_measured_fraction_theta_max 0.985
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0647
_diffrn_reflns_av_sigmaI/netI    0.0553
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -33
_diffrn_reflns_number            24776
_diffrn_reflns_theta_full        28.30
_diffrn_reflns_theta_max         28.30
_diffrn_reflns_theta_min         1.60
_exptl_absorpt_coefficient_mu    2.544
_exptl_absorpt_correction_type   SADABS
_exptl_crystal_colour            Dark_blue
_exptl_crystal_density_diffrn    2.346
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Blocks
_exptl_crystal_F_000             2728
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.08
_refine_diff_density_max         1.156
_refine_diff_density_min         -1.585
_refine_diff_density_rms         0.004
_refine_ls_extinction_coef       0.0078(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.975
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     282
_refine_ls_number_reflns         4853
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.975
_refine_ls_R_factor_all          0.0947
_refine_ls_R_factor_gt           0.0686
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0815P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1396
_refine_ls_wR_factor_ref         0.1640
_reflns_number_gt                2714
_reflns_number_total             4853
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic011124v_2.cif
_cod_data_source_block           try
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to the built-in table from CIF Core
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_database_code               4317880